| ||Format||Pages||Price|| |
|9||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||9||$52.00||  ADD TO CART|
|Standard + Redline PDF Bundle||18||$62.00||  ADD TO CART|
Significance and Use
4.1 This test method is designed to provide load versus deformation response of plastic films under essentially multi-axial deformation conditions at impact velocities. This test method further provides a measure of the rate sensitivity of the plastic films to impact.
4.2 Multi-axial impact response, while partly dependent on thickness, does not necessarily have a linear correlation with specimen thickness. Therefore, results should be compared only for specimens of essentially the same thickness, unless specific responses versus thickness formulae have been established for the plastic films being tested.
4.3 For many plastic films, it is possible that a specification exists that requires the use of this test method, but with some procedural modifications that take precedence when adhering to the specification. Therefore, it is advisable to refer to that material specification before using this test method. Table 1 of Classification System lists the ASTM materials standards that currently exist.
4.4 The values obtained by this test method are highly dependent on the method and conditions of film fabrication as well as the type and grade of resin. Results can vary significantly, depending upon sample quality, uniformity of film gage, die marks, contaminants, and so forth.
1.1 This test method covers the determination of puncture properties of plastic films, over a range of test velocities.
1.1.1 ASTM Terminology Standard has defined film as having a thickness not greater than 0.25 mm. Plastic materials having a thickness above this limit are not to be excluded from use unless shown to be rigid (see ). Test Method is the recommended method for instrumented puncture testing of rigid plastics.
1.2 Test data obtained by this test method is relevant and appropriate for use in engineering design.
1.3 The values stated in SI units are to be regarded as standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
Note 1: This test method does not closely conform to ISO 7765-2. The only similarity between the two tests is that they are both instrumented impact tests. The differences in striker, fixture, specimen geometries and in test velocity can produce significantly different test results.
1.5 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D618 Practice for Conditioning Plastics for Testing
D883 Terminology Relating to Plastics
D3763 Test Method for High Speed Puncture Properties of Plastics Using Load and Displacement Sensors
D4000 Classification System for Specifying Plastic Materials
D6988 Guide for Determination of Thickness of Plastic Film Test Specimens
E456 Terminology Relating to Quality and Statistics
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
ICS Number Code 83.140.10 (Films and sheets)
UNSPSC Code 13111200(Films)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D7192-20, Standard Test Method for High Speed Puncture Properties of Plastic Films Using Load and Displacement Sensors, ASTM International, West Conshohocken, PA, 2020, www.astm.orgBack to Top